- Nano Express
- Open Access
Using Flame-Assisted Printing to Fabricate Large Nanostructured Oxide Thin Film for Electrochromic Applications
Nanoscale Research Letters volume 15, Article number: 218 (2020)
Flame spray pyrolysis was a process to produce oxide nanoparticles in a self-sustaining flame. When the produced nanoparticles were deposited on a substrate, nanostructured oxide thin films could be obtained. However, the size of the thin film was usually limited by the fixed substrate. Here, we demonstrated that thin film with a large area could be deposited by using the moving substrate, which was precisely controlled by servo motors. As a result, the flame tip could scan over the substrate and deposit the nanoparticles on it line by line, analogues to a printing process called flame-assisted printing (FAP). As an example, nanostructured bismuth-oxide thin films with a size of up to 20 cm × 20 cm were deposited with the FAP process. The bismuth-oxide thin film exhibited a stable electrochromic property with a high modulation of 70.5%. The excellent performance could be ascribed to its porous nanostructure formed in the FAP process. The process can be extended to deposit other various oxides (e.g., tungsten-oxide) thin films with a large size for versatile applications.
FSP was a process, in which solvent with the dissolved metal precursor was sprayed into liquid droplets. Then, the droplets combust into powders in a self-sustaining flame assisted with oxygen [1,2,3,4,5]. The size of the produced powders ranges from a few nanometers to micrometers. FSP can be easily employed to produce oxide nanopowders (e.g., SiO2, TiO2, CeO2 and Al2O3) in a commercial scale [6,7,8,9]. Although the nanopowders from the FSP process can be either dropped or cast on the substrate to form the thin films, those films are usually dense with a low surface area, lacking nanofeatures. For the applications such as sensors, electrochemical and photoelectrochemical (PEC) devices, thin films with the porous structure are preferred [10,11,12]. In the above applications, the porous structure can enhance the utilization of active materials, enlarge the contact area between the electrolytes and reactants, and alleviate the stress during the lithiation. Thus, their performance can be improved. For example, LiMn2O4 films were formed by flame spray deposition and in situ annealing method . The highly porous thin film exhibited excellent cyclability. Kun et al. synthesized Li4Ti5O12 thin film for the high-performance and flexible all-solid-state battery . Tricoli et al.  extended the use of FSP for the fabrication of EC/PEC water-splitting WO3 and BiVO4 electrodes. They found that the performance of direct FSP-made photoelectrodes had been greatly improved compared with those films cast with nanopowders from the FSP process. These pioneering works enabled the use of FSP as a powerful tool to directly and rapidly fabricate functional films with good performance. However, the size of the thin film was limited by the unmoved substrate. Bismuth oxide was one of the most fascinating electrochromic materials due to its high theoretical coloration modulation and environmental friendliness [16,17,18,19,20,21,22,23,24,25,26,27]. For example, bismuth oxide thin films prepared by sputtering or vacuum evaporation were found to be new electrochromic materials [16, 24]. Furthermore, bismuth oxide thin films from the sol–gel processes showed steady electrochromic efficiency . However, their electrochromic performance should be further improved for the practical applications. In this study, we proposed a flame-assisted printing (FAP) process based on FSP to fabricate porous bismuth-oxide thin film on fluorine-doped tin oxide (FTO). The size of the thin film could reach 20 cm × 20 cm. The bismuth-oxide thin film deposited in this study exhibited excellent electrochemical properties with a coloration modulation of 70.5%. The excellent performance can be ascribed to the porous structure of thin films.
Preparation of Bismuth-Oxide Thin Films
An FAP equipment was used for the direct deposition of bismuth-oxide thin films on FTO substrates (Fig. 1a). The thin films were prepared with following steps: before the bismuth-oxide thin films were prepared by the FAP process, 20 cm × 20 cm transparent conductive FTO glass substrates which have a sheet resistance of 10 Ω/sq were cleaned by ultrasonic with acetone, deionized water, ethanol and deionized water successively. The bismuth-oxide precursor was made by heating the mixture of bismuth carbonate (1.45 g), 2-ethylhexanoic acid (20 g) and deionized water (40 μL) to 160 °C under mechanical stirring. Precursor solutions with a total Bi atom concentrations of 1 and 5 mM were prepared by dissolving bismuth-oxide precursor in 2-2-4-trimethylpentane (15 ml). This solution was supplied with a syringe pump at a rate of 2 mL/min and dispersed into a fine spray with 2.541 L/min oxygen and pressure from 0.21 to 0.33 MPa was maintained across the nozzle tip during synthesis. The spray was ignited by a supporting flame made by 0.4 L/min of high-purity methane (99.9%) and 0.4 L/min of oxygen. A substrate holder placed at a certain distance below the burner was utilized for the deposition of bismuth-oxide thin films on FTO substrates with a suitable deposition temperature of 500 °C. The FAP process continued for 6 min. More specifically, films were deposited on the FTO substrates, which were placed on a moving stage. In the end, thin-film samples were annealed at a rate of 5 °C/min from room temperature up to 550 °C in air for 2 h.
Preparation of Tungsten-Oxide Thin Films
The precursor solution was prepared by adding tungsten hexachloride (29.742 mg) to anhydrous ethanol (30 ml). The formed mixture was stirred at room temperature for 1 h. The substrate temperature was controlled in the range of 400–500 °C during the deposition.
The phase composition of the bismuth-oxide thin films was analyzed by X-ray diffraction (Bruker XRD, D8 Advance) using CuKα radiation (40 kV/30 mA). The surface morphologies of the thin films were investigated by field-emission scanning electron microscope (FESEM) with an Ultra 55 operating at 10 keV. Roughness measurements were taken using a profilometer (Bruker Contour, GT K 3D) with a cut-off value of 0.23 mm. Three different regions were evaluated in specimens to determine the roughness Ra. The EC behavior of bismuth-oxide thin films was evaluated with a standard three-electrode electrochemical cell using AutoLab 302N electrochemical workstation. The bismuth-oxide thin-film-coated FTO glass was applied as a working electrode, platinum sheet and Ag/AgCl electrode were served as a counter electrode and a reference electrode, respectively. 1 M solution of LiClO4 dissolved in propylene carbonate (PC) was used as the electrolyte. Cyclic voltammetry (CV) was carried out with the scan rate of 2 mV/s or 5 mV/s and voltage range of − 2 to 2 V and − 1 to 1 V for bismuth-oxide thin films and tungsten-oxide thin films, respectively. The optical transmittance change of the bismuth-oxide and tungsten-oxide thin films during the charging and discharging process in CV cycling was in situ recorded by a miniature spectrometer (Ocean optics, FLMT01617) at a fixed wavelength of λ = 550 nm.
Results and Discussion
The FAP device and process are illustrated in Fig. 1a, b. During the process of FAP, porous structure comes into being with the formation of nanoparticles, primary particles and large particles . The growth of nanoparticles and primary particles gives multilevel structure, while primary particle collision and large particle separation generate the porous structure . There are a lot of factors such as precursor concentration that have an impact on the final particle morphology, structure and performance. To deposit bismuth-oxide thin films, precursor solutions with concentrations of 1 and 5 mM were pumped with a speed of 2 ml/min into the nozzle and sprayed it into the droplets. They were then combusted into the oxide nanoclusters. The formed nanoclusters collided to form nanoparticles and deposited on the FTO substrate, which located at the moving stage. It was precisely controlled by the servo motors. As a result, the flame swept the substrate with a speed of 2 mm/s line by line. The gap between the neighboring lines was controlled to be 0.1 mm as indicated in Fig. 1b. The thickness of the film was controlled by the precursor concentration and repeating time. This line-by-line depositing process was analogous to a paper-printing process. Thus, we called this process as flame-assisted printing. FAP process was also used to deposit a spot when no scanning was performed and a line with the scanning process from 5 mM bismuth oxide precursor. The optical images of the deposited spot and line are shown in Fig. 1c. The size of the spot and the width of line were ~ 2 cm. Thus, FAP process may able to print an arbitrary 2D shape, though the resolution of the shape is limited to 2 cm. After the deposition, the obtained thin film was annealed at 550 °C for 2 h. X-ray diffraction (XRD) patterns in Fig. 2 revealed their crystalline and phase structures. Before the annealing, there was only α-phase (JCPD card No. 71-0465) for Bi2O3. While after 550 °C annealing, there were two new phases. They were δ-Bi2O3 phase (JCPD card No. 76-2478) and non-stoichiometric Bi2O2.33 phase (JCPD card No. 27-0051). The latter one was related to the oxygen vacancy due to annealing in the stagnant air . The above phase transition was consistent with the previous studies . The morphology of obtained bismuth-oxide thin film from 5 mM precursor was examined with a scanning electron microscopy (SEM). As shown in Fig. 3a, b, the whole structure exhibited a macroporous structure with secondary particles of several hundred nanometers. As a comparison, a thin film was also deposited from 1 mM precursor. It turned to be a solid film with the secondary particles approaching 1 μm as shown in Fig. 3c, d. The difference in the concentrations of the precursor solution apparently caused the change of morphology. And according to the large-scale characterization by using a profilometer, the mean Ra value of the Bi2O3 thin film from 5 mM precursor was measured to be 29 ± 2 nm (Fig. 3e), which was consistent with SEM analyses. Under high concentration, particles easily collided with each other and then branched secondary particles deposited on the substrates. While under low concentration, the primary particle was small enough to fill the gaps among the deposited particles. The morphology of the thin film appeared less porous. Thus, the morphology and pore structure of the thin film can be tubed with the concentration of the precursor in the FAP process. In addition, the further research on the influence of deposition time on film thickness was carried out. SEM images of the cross sections of the films for deposition times of 6 min, 12 min and 24 min are shown in Fig. 4. Their thicknesses increased with the time. Thus, FAP process also could control the thicknesses of the film by varying the deposition time.
The electrochromic property of the bismuth-oxide thin film from the 5 mM precursor was further investigated. The color of the thin film changed from light yellow in the bleached state to black in the colored state as shown in its optical image (Fig. 5a, inset). The optical spectra further revealed that the transmission was in a range of 75–100% at the bleached state, while at the colored state, the transmission of the thin film was in a range of 10%–30%. The CV curve (Fig. 5b) indicated that there were a cathodic peak at − 1.3 V and two anodic peaks at 0.1 V and 1.2 V, which are typical for the lithium intercalation of lithium ions into the bismuth-oxide structure forming LixBi2O3 while charging followed by reversible deintercalation of LixBi2O3 back to Bi2O3 during discharging, due to the Bi2O3/LixBi2O3 redox reaction. It corresponded to the following reaction :
The stable redox couple reactions of bismuth oxide cause the electrode to perform with good reversibility and demonstrate good stability by hardly altering shape, size and position of its anodic and cathodic peaks. The sharp and well-defined peaks indicate fast ion de- and insertion. The CVs in Fig. 5b of bismuth-oxide thin-film electrodes show the characteristic behavior of two-step extraction (peaks at 0.1 V and 1.2 V) and insertion (peak at − 1.3 V) of the lithium ions in deposit with uniform grain size indicating a successful film formation and densification took place. All electrodes show uniformity in particle sizing after successful film preparation. It indicates that the quality of the surface after heat treatment allows homogeneous porous layer stacking. However, the long-term cyclic stability of this bismuth-oxide thin-film electrode is not as good as expected due to poor adhesion to the FTO substrate. We leave improving this cyclic stability by adjusting the precursor concentration and annealing temperature as our future work.
The time-dependent optical transmittance of the bismuth-oxide thin films was in situ recorded during the CV measurement, as shown in Fig. 5c. The transmittance wavelength was set at 550 nm, which was highly sensitive to human eyes . After the first cycle, the maximum and minimum transmittances were 80.7% and 10.2%, respectively. Both transmittance values at the bleached state and colored state were kept stably. The minimum transmittance at the colored state and the maximum transmittance at the bleached state were recorded as Tc and Tb, respectively. Then optical contrast ΔTλ=550 nm was defined as ΔT = Tb − Tc. It is obvious that the bismuth-oxide thin film had a large optical contrast beyond 70%. The thin films had a slight optical degradation during the 2nd, 3rd and 4th cycles. The difference between colored and bleached states can be seen. This is mainly caused by the degradation in the reaction [17, 32], and the porous structure leads to an incomplete reaction . Here, EC response time, T0.5, is defined as the time at which the optical transmittance reaches 50% of the coloration/bleach state at the wavelength of 550 nm. As shown in Figs. 5c and 6b, T0.5 = 120 s for bismuth-oxide thin film deposited from 5 mM precursor solution and T0.5 = 300 s for bismuth-oxide thin film deposited from 1 mM precursor solution, respectively. The faster bleach rate could be ascribed to its porous nanostructure formed in the FAP process. Conventionally, coloration efficiency η (CE) is used to judge the EC performance with the following formula :
where Tb and Tc are the bleached and colored transmittance values at a given wavelength as mentioned above, ΔOD is the difference of optical density and Q is the corresponding inserted/extracted charge density. In this work, charge densities are calculated from the CV curves. The CEs of bismuth-oxide thin film were all larger than 10.0 cm2/C as shown in Fig. 5d. The CEs of bismuth-oxide thin film from 5 mM precursor were nearly the same as ones from the sol–gel derived thin film  and much higher than that of 3.7 cm2/C reported in ref . As for the bismuth-oxide thin film deposited from 1 mM precursor solution, the anodic and cathodic peaks were broadened, as shown in Fig. 6a. A significant peak broaden in anodic coloring was usually observed when the precursor solution concentration was far below 5 mM. This can be explained by the lower concentration which caused less solid/solid interfaces to the composite film due to the less porous structure . Meanwhile, the optical contrast was only 30–40% (Fig. 6b), and CE was 2.7–3.4 cm2/C. Compared with the thin film from 5 mM precursor solution, the poorer performance could be ascribed to the relatively solid nature of the thin film. In the electrochemical reaction, the electrolyte had less contact area with the active material. Thus, less active material participated in the reaction. Moreover, the degradation was obvious during the subsequent cycle due to the structure’s instability, which was caused by the change of the volume of the thin film in the reaction, while porous structure in the thin film from 5 mM solution could accommodate such change.
When the FAP equipment is extended to the synthesis of other oxides such as tungsten oxide as mentioned, the SEM image (Fig. 7a) exhibited the microstructure of the deposited tungsten-oxide thin film, while the precursor concentration is 2.5 mM. It had secondary particles, which aggregated a lot of spherical primary particles, which forms the cauliflower structure. More specifically, it appears that secondary particles are larger and less porous than the bismuth-oxide thin film from 5 mM precursor. There are anodic and cathodic peaks at 0.1 and − 0.5 V, which is typical for the lithium deintercalation and intercalation (Fig. 7b). Coloration/bleach in WO3 thin films is due to the insertion and extraction of lithium ion, following the reaction below :
In WO3 thin film, the inserted electrons reduce some W6+ ions to W5+ and polarize their surrounding lattice to form small polarons which cause the optical absorption. In bismuth-oxide thin film, the coloration/bleach may follow the same mechanism. However, the unstable chromatic properties may be caused by the stress build-up due to volume change or dissolution of LixBi2O3 in the electrolyte during the reaction. The detachment of bismuth-oxide thin film from FTO substrates was often found after several coloration/bleach cycles. The bleached and colored states kept stable in 4 cycles (Fig. 7c). The chromatic property of tungsten oxide is more stable than bismuth oxide [16, 17, 35,36,37,38,39]. The optical contrast was around 35%. It was relatively low, but not lower than bismuth-oxide thin film deposited from 1 mM precursor. To get a higher value, the thickness of tungsten-oxide thin film should be increased. The first coloration efficiency of tungsten oxide was 3.4 cm2/C, which was nearly the same as the data reported  and between the bismuth-oxide thin films from 1 and 5 mM precursor. Magnetic sputtering, pulsed laser deposition and chemical vapor deposition are several popular coating methods. They can be used to produce high-quality thin film with a thickness precision of several nanometers. However, all of them are difficult to produce large-area thin films due to the size limitation of deposition chamber. While FAP process can easily prepare large samples, it can be operated in the open atmosphere. Meanwhile, though the process cannot control the thickness very precisely, it can adjust the morphology of the thin film for the specific applications. The result above indicated that FAP could tune the nanostructure of the deposited film by precursor concentration, which further influenced its electrochromic performance.
Conclusion and Outlook
Large-area bismuth-oxide thin films were successfully prepared by a FAP process. The morphology of the thin films could be tuned with the deposition parameters such as the concentration of the precursor solution. The bismuth oxide with porous nanostructure exhibited excellent electrochromic property, with a maximum optical contrast of 70.5% and a coloration efficiency above 10.0 cm2/C. This FAP process can be extended to the synthesis of other porous nanostructured materials for applications in energy storage and conversion.
Availability of data and materials
All data generated or analyzed during this study are included in this published article.
Flame spray pyrolysis
Fluorine-doped tin oxide
Field-emission scanning electron microscope
Scanning electron microscopy
Kammler HK, Mädler L, Pratsinis SE (2001) Flame synthesis of nanoparticles. Chem Eng Technol 24:583–596
Mädler L, Kammler HK, Mueller R, Pratsinis SE (2002) Controlled synthesis of nanostructured particles by flame spray pyrolysis. J Aerosol Sci 33:369–389
Teoh WY, Amal R, Mädler L (2010) Flame spray pyrolysis: an enabling technology for nanoparticles design and fabrication. Nanoscale 2:1324–1347
Hu Y, Ding H, Li C (2011) Preparation of hollow alumina nanospheres via surfactant-assisted flame spray pyrolysis. Particuology 9:528–532
Heine MC, Mädler L, Jossen R, Pratsinis SE (2006) Direct measurement of entrainment during nanoparticle synthesis in spray flames. Combust Flame 144:809–820
Jang HD, Chang H, Suh Y, Okuyama K (2006) Synthesis of SiO2 nanoparticles from sprayed droplets of tetraethylorthosilicate by the flame spray pyrolysis. Curr Appl Phys 6:e110–e113
Akurati KK, Vital A, Dellemann J-P, Michalow K, Graule T, Ferri D, Baiker A (2008) Flame-made WO3/TiO2 nanoparticles: relation between surface acidity, structure and photocatalytic activity. Appl Catal B 79:53–62
Mädler L, Stark WJ, Pratsinis SE (2011) Flame-made ceria nanoparticles. J Mater Res 17:1356–1362
Tangsir S, Hafshejani LD, Lähde A, Maljanen M, Hooshmand A, Naseri AA, Moazed H, Jokiniemi J, Bhatnagar A (2016) Water defluoridation using Al2O3 nanoparticles synthesized by flame spray pyrolysis (FSP) method. Chem Eng J 288:198–206
Yuan D, Zeng J, Kristian N, Wang Y, Wang X (2009) Bi2O3 deposited on highly ordered mesoporous carbon for supercapacitors. Electrochem Commun 11:313–317
Cho JS, Ko YN, Koo HY, Kang YC (2010) Synthesis of nano-sized biphasic calcium phosphate ceramics with spherical shape by flame spray pyrolysis. J Mater Sci - Mater Med 21:1143–1149
Wang SX, Jin CC, Qian WJ (2014) Bi2O3 with activated carbon composite as a supercapacitor electrode. J Alloys Compd 615:12–17
Chew SY, Patey TJ, Waser O, Ng SH, Büchel R, Tricoli A, Krumeich F, Wang J, Liu HK, Pratsinis SE, Novák P (2009) Thin nanostructured LiMn2O4 films by flame spray deposition and in situ annealing method. J Power Sources 189:449–453
Gockeln M, Glenneberg J, Busse M, Pokhrel S, Mädler L, Kun R (2018) Flame aerosol deposited Li4Ti5O12 layers for flexible, thin film all-solid-state Li-ion batteries. Nano Energy 49:564–573
Tran-Phu T, Chen H, Bo R, Di Bernardo I, Fusco Z, Simonov AN, Tricoli A (2019) High-temperature one-step synthesis of efficient nanostructured bismuth vanadate photoanodes for water oxidation. Energy Technology 7:1801052
Shimanoe K, Suetsugu M, Miura N, Yamazoe N (1998) Bismuth oxide thin film as new electrochromic material. Solid State Ionics 113–115:415–419
Yu J, Shi J, Yu S (2017) The electrochromic behavior of Bi2O3 thin film prepared by sol–gel technique. J Sol-Gel Sci Technol 84:239–245
Zuo W, Zhu W, Zhao D, Sun Y, Li Y, Liu J, Lou XW (2016) Bismuth oxide: a versatile high-capacity electrode material for rechargeable aqueous metal-ion batteries. Energy Environ Sci 9:2881–2891
Sammes NM, Tompsett GA, Näfe H, Aldinger F (1999) Bismuth based oxide electrolytes—structure and ionic conductivity. J Eur Ceram Soc 19:1801–1826
Jiang S, Wang L, Hao W, Li W, Xin H, Wang W, Wang T (2015) Visible-light photocatalytic activity of S-doped α-Bi2O3. J Phys Chem C 119:14094–14101
Schmidt S, Kubaski ET, Volanti DP, Sequinel T, Bezzon VDN, Beltrán A, Tebcherani SM, Varela JA (2015) Effect of pressure-assisted heat treatment on photoluminescence emission of α-Bi2O3 needles. Inorg Chem 54:10184–10191
Lu Y, Zhao Y, Zhao J, Song Y, Huang Z, Gao F, Li N, Li Y (2015) Induced aqueous synthesis of metastable β-Bi2O3 microcrystals for visible-light photocatalyst study. Cryst Growth Des 15:1031–1042
Gujar TP, Shinde VR, Lokhande CD, Han S-H (2006) Electrosynthesis of Bi2O3 thin films and their use in electrochemical supercapacitors. J Power Sources 161:1479–1485
Gotić M, Popović S, Musić S (2007) Influence of synthesis procedure on the morphology of bismuth oxide particles. Mater Lett 61:709–714
Zhao X, Liu H, Qu J (2011) Photoelectrocatalytic degradation of organic contaminants at Bi2O3/TiO2 nanotube array electrode. Appl Surf Sci 257:4621–4624
Zhu BL, Zhao XZ (2006) Study on structure and optical properties of Bi2O3 thin films prepared by reactive pulsed laser deposition. Opt Mater 29:192–198
Ziegler JP, Howard BM (1995) Applications of reversible electrodeposition electrochromic devices. Sol Energy Mater Sol Cells 39:317–331
Johannessen T, Pratsinis SE, Livbjerg H (2000) Computational fluid-particle dynamics for the flame synthesis of alumina particles. Chem Eng Sci 55:177–191
Giesen B, Wiggers H, Kowalik A, Roth P (2005) Formation of Si-nanoparticles in a microwave reactor: comparison between experiments and modelling. J Nanopart Res 7:29–41
Higaki K, Kudo S, Ohnishi H (1998) Highly selective NO detection using Bi2O3-based materials. Electrochem Solid-State Lett 1:107–109
Arvizu MA, Wen R-T, Primetzhofer D, Klemberg-Sapieha JE, Martinu L, Niklasson GA, Granqvist CG (2015) Galvanostatic ion detrapping rejuvenates oxide thin films. ACS Appl Mater Interfaces 7:26387–26390
Wen R-T, Arvizu MA, Morales-Luna M, Granqvist CG, Niklasson GA (2016) Ion trapping and detrapping in amorphous tungsten oxide thin films observed by real-time electro-optical monitoring. Chem Mater 28:4670–4676
Yu XQ, Wang RI, He Y, Hu YS, Li H, Huang XJ (2010) Electrochromic behavior of transparent Li4Ti5O12/FTO electrode. Electrochem Solid State Lett 13:J99–J101
Roeder M, Beleke AB, Guntow U, Buensow J, Guerfi A, Posset U, Lorrmann H, Zaghib K, Sextl G (2016) Li4Ti5O12 and LiMn2O4 thin-film electrodes on transparent conducting oxides for all-solid-state and electrochromic applications. J Power Sources 301:35–40
Yang T-S, Lin Z-R, Wong M-S (2005) Structures and electrochromic properties of tungsten oxide films prepared by magnetron sputtering. Appl Surf Sci 252:2029–2037
Wang J, Khoo E, Lee PS, Ma J (2008) Synthesis, assembly, and electrochromic properties of uniform crystalline WO3 nanorods. J Phys Chem C 112:14306–14312
Jiao Z, Sun XW, Wang J, Ke L, Demir HV (2010) Hydrothermally grown nanostructured WO3 films and their electrochromic characteristics. J Phys D Appl Phys 43:285501
Lee SH, Deshpande R, Parilla PA, Jones KM, To B, Mahan AH, Dillon AC (2006) Crystalline WO3 nanoparticles for highly improved electrochromic applications. Adv Mater 18:763–766
Sallard S, Brezesinski T, Smarsly BM (2007) Electrochromic stability of WO3 thin films with nanometer-scale periodicity and varying degrees of crystallinity. J Phys Chem C 111:7200–7206
This work was supported by National Key Research and Development Program of China (2017YFA0204600) and the National Science Foundation of China programs (Nos. U1703128, U1503292).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Fan, H., Yan, W., Ding, Y. et al. Using Flame-Assisted Printing to Fabricate Large Nanostructured Oxide Thin Film for Electrochromic Applications. Nanoscale Res Lett 15, 218 (2020). https://doi.org/10.1186/s11671-020-03450-6
- Flame-assisted printing
- Bismuth oxide
- Thin films